Goetzendorf-Grabowska B, Karaszewska A, Vlasenko VI., Arabuli
AT. Bending Stiffness of Knitted Fabrics Comparison of Test
Methods.FIBRES & TEXTILES in Eastern Europe 2014; 22, 1(103):
Bending Stiffness of Knitted Fabrics Comparison of Test
Bogna Goetzendorf-Grabowska, Agnieszka Karaszewska,
*Victoria I. Vlasenko, *Arsenii T. Arabuli
Textile Research Institute, Scientific Department
of Unconventional Technologies and Textiles, ul. Brzeziska 5/15,
92-103 d, Poland
E-mail: [email protected]
*Kiev National University of Technologies & Design,
2N-Danchenko St.korp. 1, 132 01011, Kiev, Ukraine
AbstractThe bending stiffness of a textile is a feature
determining comprehensive indicators such as fabric drapability and
handle. Most methods of assessing the bending stiffness of textiles
are based on the principle of the determination of the strain and
force dependence. The simplest are methods involving the
unidirectional straining force, which do not consider the
anisotropy of the fabrics physical properties. However, methods
that allow the deter-mination of multi-directional stiffness
provide a more complete assessment. The aim of this work was to
comparatively evaluate three testing methods that utilise different
measure-ment principles. The experimental design included a
unidirectional force action (PN-73/P0431), multidirectional force
action (ASTM-D 4032-94), and bending stiffness testing by the
direct determination of Youngs modulus by the method used at Kiev
University. The methods analysed were assessed by statistical
tests. Knitted fabrics with a net stitch were used as the test
Key words: test methods, bending stiffness, statistic test.
ing. The most popular gravimetric meth-ods are those using the
determination of the bending length as a measure of the interaction
between fabric weight and stiffness [7 - 11]. One of them is
Pierces Heard Loop Test . This principle is used by ASTM 
and PN . A known example of the bending length prin-ciple is
the Cantilever Test for Stiffness [13, 14].
The determination of fabric stiffness is also included in KES
(Kawabata Evalua-tion System) and Handle-O-Meter Tester [15 -
The simplest and most available methods are based on the
unidirectional action of the straining force action [19, 20]. In
view of the anisotropy of physical properties of textile fabrics,
the method of the uni-directional action of force usually takes
into account three basic directions of the fabric (longitudinal,
transversal and the bias- 45 (deg) to the samples axis). This is,
however, a simplification that does not include the anisotropy
character. The methods that determine multidirectional stiffness
give a more complete assess-ment [21 - 26].
An interesting method has been devel-oped at the Kiev National
University of Technologies & Design (Ukraine) for the dynamic
determination of elasticity mod-ulus (Ed) based on a theory that
elasto-plastic bodies subjected to cyclic sinusoi-dal stresses
reach a state of equilibrium after a number of cycles, which is a
func-tion of the structures dynamic proper-ties . A similar
method of measuring Youngs module for fibre was developed by Polish
Isotropic materials are characterised by one Youngs modulus,
while for aniso-tropic materials such as textiles, the num-ber of
elasticity coefficients is higher than one, which are connected
with the main anisotropy directions. Due to the com-plex fibre
structure, the action of external forces results in complicated
phenomena of mechanical properties that cannot be included in the
classic theory of an elas-tic or plastic body. Taking into account
the components of strain occurring under the influence of force,
fibres are defined as anisotropic visco-elastic bodies . The
complexity of the fabric strain anisotropy results from the
overlapping parameters of the structures of fibres, yarns and
There are many test methods known for measuring fabric bending
stiffness, but only few of them use Youngs modulus as a basis for
measuring stiffness .
Most methods described and used in tex-tile laboratories are
based on the princi-ple of indirect stiffness assessment by
determining the dependence of strain and the force that induces
this strain. Some methods use tensile testing machines for precise
measurement of the dependence of the force and strain of flat
textile fab-rics . In view of the narrow range of the acting
forces and occurring strains, such methods allow one to obtain
results with smaller errors.
Dziworska  introduced two types of testers for measuring
bending stiffness. The first type of testers measure the fab-ric
strain under its own weight (gravita-tion method), whereas the
other testers are based on the measurements of forces, bending
moments or energy during bend-
n IntroductionThe stiffness of some fabrics constitutes the
basic feature determining their suit-ability for a specific use.
The bending stiffness of textiles has become a funda-mental
property in determining the com-plex parameter of fibre or fabric
drapabil-ity and handle.
The drapeability of textiles in physical terms is a result of
mutual interaction between the bending stiffness and fabric weight
Generally rigidity is defined as the capa-bility of a material
to resist strain under the influence of different forces such as
compression, uniaxial tension, bending, simple shearing or
vibration . For elastic bodies, in most strains, stiffness is
characterised by Youngs modulus (E), determined as the modulus of
linear strain ability . This is a parameter de-termining fabric
elasticity, which makes the material linear strain dependent on
stress occurring in it according to the de-pendence:
E = /, N/m2 (1)
where: - relative linear strain, - stress
The stiffness rigidity (G) is measured by the product of modulus
(E) and the mo-ment of inertia (I) of the cross-section in relation
to the neutral axis passing through the middle of the cross-section
according to the following formula:
G = E I, N (2)
This dependence constitutes a theoretical basis for the physical
determination of the bending rigidity parameter .
FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No.
The aim of this work was to comparative-ly evaluate three
selected testing methods using different measurement principles to
evaluate the bending stiffness of net-like warp knitted
The test material consisted of 10 groups of surgical netlike
warp knitted fabrics with various variants of yarn and knitting
stitches of the same fibre raw material (polyester).
The experimental design includes uni-directional force action
(PN-73/P0431) and multidirectional force action (ASTM-D 4032-94) as
well as bending stiffness testing by direct determination of Youngs
modulus by the method used at Kiev University.
Comparison of results and properties of the methods evaluated
was carried out by means of statistical tests [29 - 32].
n Experimental detailsMaterialTest materials consisted of
polyester openwork warp knitted fabrics with dif-ferent fabric and
yarn parameters. Basic fabric parameters and images of knitting
stitches are listed in Table 1 and shown in Figure 1.
To better characterise the structure of the net knitted fabrics
tested, the following parameters were determined on the basis of
microscopic analysis :Cs total - Total surface of voids - the
of surfaces of all the voids on the sample surface tested Ss in
Cs max. - Maximal surface of a single void in mm2, Figure 2.
P - Porosity - the percentage content of the total void surface
in the sample surface
P = Cs total/Ss, % (3)
The results of this analysis are listed in Table 2.
MethodsDetermination of textile fabric stiffness - Polish
Standard PN-73/P0463 This is a gravitational method based on
Pierces theory. The principle of this method consists in measuring
the bend-ing length of a sample, whose both ends are fixed in a
clamp. The freely hanging sample forms a heard loop, and the sag
length in m is the basis for determination
Table 1. Characteristics of test materials.
Symbol of knitted
Type of yarn Type of knitting stitch
g/m2 wale course
I Polyester30 dtex, f 1
Plain, double needle board stitch with combined stitches
16.3 11.8 54.0II 20.0 12.0 65.2
III Polyester56 dtex f 24 Double Plain, double needle board
stitch with network structure
22.1 11.2 62.6
IV Polyester56 dtex f 24 Single 21.8 10.9 41.9
V Polyester56 dtex f 24 Double Plain, three needle board, stitch
with network structure
16.9 11.6 67.5
VI Polyester56 dtex f 24 Single 18.0 12.1 49.5
Polyester30 dtex f 1
Plain, double needle board stitch with network structure
19.6 10.7 22.2VIII 24.6 11.8 27.2IX Plain, double needle board
with network structure 28.2 9.5 24.7
X 29.7 11.2 28.3
Figure 1. Images of knitting stitches.
Figure 2. Surface of a single void of an exemplary sample.
Plain, double needle board stitch, with combined stitches
III IV IX X
Plain stitch, double needle board with a network structure
Plain, three needle board stitch with a network structure
Plain, double needle board stitch
Sample VCs max: 3.118 mm2
45FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No.
nance occurs. The numerical value of Tp appears on the frequency
meter at the moment of resonance.
The low frequency generator determines the frequency of
oscillation at resonance, and the frequency meter gives the
nu-merical value of the period, Tp. It is the numerical value of
the period that is used for further calculations.
Schema of the Stiffness Tester, shown in Figure 4.
The force F, N required to push out a sample along the holes
axis at a length of 57 mm is a result of measurement. An electronic
meter with a memory element allows a read-out of 10 measurements
with statistics. Stiffness measurements were performed according to
the proce-dure of the above standard for sample size n = 10.
Dynamic modulus of elasticity Ed (method UDM-1) Tests of
bending stiffness based on the determination of Youngs modulus were
carried out at Kiev National University of Technology & Design.
The UDM-1 apparatus operating on the principle of inducing the
resonance of the samples longitudinal vibration and measuring the
vibration frequency at the moment of equilibrium allows one to
determine the elasticity modulus. A scheme of this ap-paratus is
shown in Figure 5.
The dynamic modulus of elasticity is de-termined on the basis of
the sample vi-bration and parameters (dimension and weight). The
samples were loaded with a given mass MI depending on the type of
fabrics tested. Under the influence of this load samples were
investigated. Free longitudinal damped oscillations occur in the
sample due to the given load. Oscilla-tions depend on the
properties of the ma-terials, in particular its elasticity.
To determine the oscillation period, Tp, one must determine the
oscillation frequency of the sample. This can be achieved by
turning the handle of the generator at the frequency which
of the bending length. Figure 3 shows the scheme of
The loop length m allows determination of the bending length c
on the basis of tabulated values c = f (m)
Based on the measurement results, the bending stiffness, G, is
G = 10-6mFc3g, mNm (mNm - milinewton meter) (4)
where: mF fabric weight, g/m2, c bending length, cm, g
acceleration of gravity, m/s2.
Bending modulus q is calculated from the formula:
q = 1.2104G/h, kPa (5)
where: h sample thickness, mm.
Measurements are separately performed for the longitudinal and
transversal direc-tions and the result is the geometrical av-erage
of both measurements.
For each sample and each direction the sample size was n =
All calculations was made in agreement with formula of PN
ASTM D 4032 92, Standard test method for measuring fabric
stiffness by the circular bend procedure This is a method of
multidirectional force action to a specified strain. Its principle
of measurement consists in determining the maximal force of a
mandrel causing a simultaneous multidirectional fabric strain by
pushing a sample through the tester table hole. Stiffness
measurements according to this method were performed by means of a
Table 2. Structural parameters of the knit-ted fabrics
Symbol of knitted
Porosity Paverage value, %
Max clearance surface
Cs max., mm2
I 46.6 0.14II 35.3 0.05III 55.7 1.70IV 69.1 1.91V 50.9 4.77VI
65.2 3.12VII 73.9 1.04VIII 71.0 0.89IX 74.8 1.19X 71.2 0.86 Figure
3. Scheme of measurement by the loop method; 1) clamps, 2)
scale, 3) fabric sample, m) loop length .
Figure 4. Digital pneumatic stiffness tester .
Figure 5. Operating principle of UDM-1 instrument.
Sample in clamps
Vibration induction system
Low frequency generator
Platform + sample
FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No.
On the Oscillograph one can see the moment when resonance is
The elasticity modulus Ed is calculated from the following
Mlld = , N/m2 (6)
where: l0 - operating sample length in m, l - load weight in kg,
Sc - surface of sample cross-section in m2, - vibra-tion period
corresponding to resonance moment in s.
The bending stiffness Rb can be deter-mined using the formula of
Rb = Ed.I, Nm2 (7)
The moment of inertia I for a rectangular sample cross-section
3bhI = , m4 (8)
where: b - sample width, h - sample thickness.
Measurements are carried out on rec-tangular samples of width =
30 mm and length = 100 mm cut out in lon-gitudinal and transversal
directions, and at an angle of 45. The load mass MI = 0.0407 kg.
The measurement result is an average value of sample size n =
The calculations were performed in ac-cordance with the
methodology set .
The program developed for mathemati-cal processing, which is
linked to the ap-paratus, allows one to analyse the elas-ticity
modulus in each direction (multi-directionally), within an angle
range of 0 - 360, using the interpolation method .
This processing results in a polar dia-gram of modulus Ed as a
function of the inclination angle (angle between the samples axis
and the direction of vibra-tion). The representation of Ed = f
(angle) within the range of 0 - 360 in the form of a linear diagram
shows that in view of the mirror reflections of curves in
succes-sive ranges of the polar diagram, it is enough to analyse
the variability of Ed values or angles at 0 90. Ed assessment takes
into account the anisotropic proper-ties of textiles. Figure 6
shows examples of polar and linear diagrams.
In the method described above, the result of stiffness
assessment consists of the av-eraged Ed values for the basic
directions (longitudinal, transversal and bias direc-tion - 45
(deg) to the samples axis) and the polar diagram.
Statistical analysis Statistical procedures were carried out
with the use of the STATISTICA 8 pro-gram .
The following tests were performed:n Descriptive statistics M -
- standard deviation, SV coefficient of variation, shape of
n Analysis of variance:
n one-way ANOVA, a technique used to compare the means of groups
(ten groups of knitted fabrics)
n post hoc statistics in groups, results of multiple comparisons
peer-to-peer (45 pairs of groups). Signifi-cant difference between
pairs at the level = 0.05 ; tests for distribution normality RIR
Tukeys; without normal distribution Krusk-Wal-lis H.
n Spearmans rank correlation
To check the comparability of results of the methods analysed
Spearmans rank correlation coefficients between stiffness results
of the methods were calculated.
n Test power analysis. Performing pow-er analysis and sample
size estimation is an important aspect of experimental results [29
- 32] The power of a test is determined by three factors: the
sam-ple size, level, and effect size. The levels of effect size
determined by Co-hen [31, 32] and used for test power calculation
are listed in Table 3.
Figure 6. Diagrams of Ed as a function of the inclination angle
of the samples axis to the direction of vibration (sample VII).
Table 3. Levels of effect size.
Effect sizePower levels
Small Medium LargeNormal distributionf-tests ANOVA 0.10 0.25
Without a normal distributiont-test on means
0.20 0.50 0.80
0 90 180 270 360Inclination angle,
0 - 9090 - 180180 - 270270 - 360
47FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No.
The test power for the groups analysed was calculated using
level = 0.05; effect sizes at a medium and large level of power;
tests for distribution normality f - Anova test; without normal
distribu-tion - t-test on means.
The test power for the sample size of the methods was calculated
and the number of measurements required for the accept-able test
power level 0.8 0.9 was ana-lysed [31, 32].
Analysis of the variability of directional bending stiffness
based on the diagrams EdUsing the possibility of presenting the
val-ues of elasticity modulus (Ed) (UDM-1) in the form of a diagram
comprising the whole range of the force direction 0 - 90, an
additional analysis of the mod-ulus as a function of the direction
of the force was made.
n Results and discussionStatistical analysisBasic descriptive
statistic parametersThe test results of bending stiffness and the
basic descriptive statistic parameters are listed in Table 4.
Test of normality distribution show that only method UDM-1 has a
normality shape of distribution.
Analysis of varianceOne-way ANOVA. In the results of the
analysis of variance at the level of prob-ability p < 0.05,
marked effects were significant. It means that the averages of
groups differ significantly.
Post hoc statistics in groups, multiple comparisons
peer-to-peer. Analysis of results of multiple comparison
peer-to-peer (45 pairs of groups) tests show that significant
differences occur only in 40 - 50% of all the groups tested. Among
the methods under comparison, it is the UDM-1 (Rb) method that
better differen-tiates the groups tested than the remain-ing two
The results of multiple comparisons by RIR Tukeys test and
Krusk-Wallis H. test are listed in Table 5.
Analysis of these results shows that significant differences
occur only in 40 - 50% of all the groups tested. Among the methods
under comparison, it is the UDM-1 (Rb) that better
Table 4. Test results of bending stiffness.
Symbol of knitted fabric group
PNG, mNm; n = 20
ASTMF, N; n = 10
UDM-1Rb, Nm2, n = 15
M SD CV,% M SD CV,% M SD CV, %I 8.02 0.61 7.60 1.67 0.05 3.50
2.39 1.22 51.0II 4.81 1.50 31.2 1.73 0.05 14.3 3.00 2.55 84.9III
3.28 0.44 13.4 1.52 0.18 12.1 2.02 1.13 56.0IV 3.77 0.50 13.3 1.52
0.22 14.8 0.91 0.65 71.1V 3.71 0.53 14.3 1.35 0.10 7.50 2.49 0.68
27.6VI 3.08 0.37 12.0 1.40 0.31 23.4 2.16 1.23 56.9VII 2.11 0.38
18.0 0.51 0.13 26.1 0.56 0.20 37.3VIII 2.29 0.27 11.8 0.59 0.13
22.0 0.51 0.13 26.4IX 1.79 0.76 42.5 0.51 0.11 21.8 0.47 0.49 104X
2.08 0.25 12.0 0.58 0.13 22,0 0.56 0.57 102
Table 5. Results of multiple comparisons (45 pairs of groups).
Significant difference be-tween pairs at the level p = 0.05.
Method Significant differences in number of pairsSignificant
of all the groups tested, %
PN 18 40
ASTM 18 40 UDM-1 23 50
Figure 7. Results of Spermans rang correlation between methods
FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No.
the groups tested than the remaining two methods.
Spearmans rank correlationConsidering the different indicators
and value level of the methods under analy-sis, Spearmans rank
correlation was used for their comparison. The results of Spearmans
rank correlation coefficients are shown in Figure. 7. This
Table 6. Results of power test analysis.
Level of power PN ASTM UDM-1
Sample size, n 20 10 15
Effect sizeMedium t = 0.50 f = 0.25Large t = 0.80 f = 0.40
Power calculatedMedium 0.15 0.09 0.45Large 0.31 0.17 0.98
Sample size required, nMedium 189 189 37Large 74 74 15
Figure 8. Image of diagrams for various groups of knitted fabric
stitch: a) plain, double needle board stitches (velvet, chain), b)
plain stitch, double needle board with a network structure; c) V,
VI plain, three needle board stitch with a network structure; VII,
VIII plain, double needle board stitch.
49FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No.
show that a high level of correlation co-efficients, R > 0.7,
between all methods compared means that they give compa-rable
revaluation of the bending stiffness of the fabrics tested. It is
suitable to com-pare estimates of bending stiffness for re-sults
Rb, G and F but only in a specified range.
Test power analysis Results of the test power calculated at the
acceptance level of effect size (STATISTICA 8 program) are
presented in Table 6.
This results show that only the UDM-1 method reached a
satisfactorily large lev-el of test power - 0.9088 and has a
suffi-cient sample size n = 15. Residual meth-ods did not achieve
satisfactory results of power - 0.8 - 0.9 at a large and medium
level and could not bring results with a statistically significant
difference. On the other hand the required sample size cal-culated
for the standardised methods is difficult to use in practice.
Analysis of the variability of the directional bending stiffness
based on the diagrams Ed Diagrams of all the samples tested are
shown in Figure 8.
The presentation of diagrams Ed as a function of the axis slope
of the sample to the direction of force action allows one to
isolate some groups corresponding to the stitch of the nets tested
and to compare them within these groups. The shape of curves
depends on the repeat determining stitch, clearance size, yarn
thickness and structure.
Knitting of the first groups I and II, (Fig-ure 1, Table 2) with
combined stitches (chain, velvet) shows increasing stiff-ness
versus the angle up to the maximal double Ed value for the parallel
direction to wales (90). At the same time, these groups show the
greatest anisotropy of stiffness.
In the case of groups with plain net stitches, values of the
elasticity modulus are sinusoidally changed, reaching their maximum
within the range of 30 - 50.
Analysing these diagrams, one can as-sess the character of
bending stiffness for the specified fabric stitch on the basis of
modulus values. Knitting with combined stitches (I and II) is
characterised by the greatest stiffness among the knitting
ed, which is shown at about 90, i.e. in the direction of
Groups with plain two-needle net stitches (III, IV, IX and X),
Figure 8.b reach their maximal stiffness within the range of 30 -
Groups with plain three-needle and two-needle stitches and with
different yarns and numbers of knitted loops (V, VI, VII and VIII),
Figure 8.c constitute nets with the best multi-directionally
equalised stiffness due to the smallest differences in the modulus
versus the angle.
n Conclusions The aim of this work was to compara-tively
evaluate three selected testing methods using different measurement
principles and choose the best to evalu-ate the bending stiffness
of net-like warp knitted fabrics. The experimental de-sign included
unidirectional force action (PN-73/P0431) and multidirectional
force action (ASTM-D 4032-94) as well as bending stiffness testing
by direct determination of Youngs modulus (E) used for calculations
of bending stiffness (method UDM-1). Comparison of results and
evaluating properties of the methods was carried out by means of
statistical tests with the use of the STATISTICA 8 program.
Results of the analysis of variance show that the one-way ANOVA
for the three methods tested confirmed differences between the
average values of bending stiffness for all the groups. Results of
multiple comparisons peer-to-peer show that significant differences
occur only in 40-50% of all the groups tested. Among the methods
under comparison, it is the UDM-1 (Rb) that better differentiates
the groups tested than the remaining two . The high level of
Spearmans rank cor-relation coefficients, R > 0.7, between all
methods compared is well suited to com-pare estimates of bending
stiffness for results Rb, G and F, but only in a speci-fied range.
Results of the test power show that only the UDM-1 method reached a
satisfactorily large level of test power 0.9088 and has sufficient
sample size n = 15. Standardised methods in PN and ASTM did not
achieve satisfactory re-sults of power 0.8 - 0.9 at a large and
me-dium level, and the required sample size calculated for them is
difficult to use in practice. Analysing the variability of the
directional bending stiffness based on the
diagrams (Ed), one can assess the char-acter of bending
stiffness anizotropy for the specified fabric stitch on the basis
of modulus values. In a general summary it can be concluded that
standardised meth-ods in PN and ASTM, as a comparison, can be used
in quality control, applicable in industry. Due to the possibility
of anal-ysis diagrams in many directions of force action and the
satisfactorily large level of test power, the UDM-1 method is
useful for scientific works.
AcknowledgmentsThe samples of knitted fabrics with a network
structure used in this study were prepared within research project
1242/T08 29 (2005-2008). The authors would like to thank Krzysz-tof
Raczyski, M.Sc., Project Manager, for providing the material for
investigations. The authors are also indebted to Irena Kamiska,
M.Sc. for performing microscopic analyses of the fabric
References 1. yliski T. Metrologia Wkiennicza.
WNT, 1965: 403 410. 2. Dziworska G. Przegld modeli, system-
w i metod pomiarowych sztywnoci zgi-nania paskich wyrobw
wkienniczych. Przegld Wkienniczy 2004; 8: 40-43.
3. Ostwald M. Podstawy wytrzymaoci materiaw. WPP, 2007: 93
4. yliski T. Nauka o Wknie. WPLiS 1958: 131 161.
5. Urbaczyk GW. Fizyka Wkna 2002: 144 196.
6. Kocik M, urek W, Krucinska I, et al. Evaluating the Bendig
Rigidity of Flat Textiles with the Use of an Instron Ten-sile
Tester. Fibres & Textiles in Eastern Europe 2005; 2: 31-34.
7. ASTM D4850-03a. Standard Terminol-ogy Relating to
8. ASTM D1388-96. Standard Test Method for Stiffness of
9. BS 3356:1990. Method for the deter-mination of bending lenght
and flexural rigidity of fabrics.
10. ISO 9073-7.1998. Test methods for non-wovens. Determination
of Bendig lenght.
11. PN-73/P-04631. Metody bada wyrobw wkienniczych. Wyznaczanie
sztywno-ci zginania. Methods of test for textiles. Determination of
12. Brown P. Measurment of Single Jersey Fabric Stiffness: A
Simple Method. Text. Res. J. 1978: 295-299.
13. Szablewski P, Kobza W. Numeryc-zna analiza testu Pierca
okrelajcego sztywno zginania wyrobw wkien-niczych. Przegld
Wkienniczy 2002; 70: 14 -17.
14. ASTM D5732-95. Standard Test Method for Stiffness of
Nonwoven Fabrics Using the Cantilever Test.
15. Ghane M, Saghafi R, Zarrebini M, Sem-nani D. Evaluation of
Bending Modulus of Needle-Punched Fabrics Using Two Simply
Supported Beam Method. Fibres
FIBRES & TEXTILES in Eastern Europe 2014, Vol. 22, No.
& Textiles in Eastern Europe 2011; 19, 4 (87): 89-93.
16. Weia M. The Theory of the Cantilever Stiffness Test. J.
Textile Inst. 1998; 80: 98 106.
17. ASTM D6828-02. Standard Test Method for Stiffness of Fabric
by the Blade/Slot Procedure.
18. Kalyanaraman AR, Sivaramakrishnan A. An electronic Fabric
Stiffness Me-ter -Performance Evaluation with the Known
Instruments. Text. Res. J. 1984; 21: 479-484.
19. Abbott NJ. The Measurement of Stiff-ness in Textile Fabrics.
Text. Res. J. 1951; 21: 435-441.
20. Sun MN. New Tester and Method for Measuring Fabrics
Stiffness and Drape. Text. Res. J. 2008; 78: 761-770.
21. De la Araujo M, Fangueiro R, Soutinho F. Improving the
stiffness of unidirec-tionally oriented weft-knitted structures for
polymer matrix composite reinforce-ment. J. Textile Ins. 2009; 9:
22. Harrabi L, Dolez PI, Vu-Khanh T, et al. Characterization of
protective Glover stiffness: Development of a multidirec-tional
deformation test method. Safety Science 2008; 46: 10251036.
23. ASTM D4032-94. Standard test Method for Stiffness of Fabrics
by the Circular Bend Procedure.
24. Vlasenko V, Kovtun S, Bereznenko N. Investigation of
Composite Textiles Visco-elastic Properties by Methods of
longitudal Resonance Vibration. In: 4th Central European Conference
Fibre-Grade Polymers, Chemical Fibres and Special Textiles. Czech
Republic 2005; 7-9 September, 217-8.
25. Owaki H. Measuring Flexural Rigidity of Fabrics by a
Vibrating Disk Method. J The Text Mach Soc Japan 1968; 12:
26. Ajeli S, Rastgo A, Gorga RE. An analysis of the bending
rigidity of warp-knitted fabrics: a comparision of experimental
results to a mechani-cal model. J. Textile Inst. 2009; 6:
27. Kostrickij WW. Mietodika i ispitatielnaja ustanowka dla
issliedowania dinamic-zeskich swojstw polimernych plienoc-znych
materiaow i wookon. Zawodska-ja aboratorija 1990; 56: 38-42.
28 Wiecek T, Konecki W. Comparative Re-search of the Dynamic
Youngs Module. Fibres Fibres &Textiles in Eastern Eu-rope 2011;
19, 4(87): 89-93.
29. Program Stat Soft Statistica 8. 30. Stat Soft. Inc.
Electronic Statistics Tex-
book. Tulsa, OK.: Statsoft. WEB, //www.statsoft. com/textbook/
31. Cohen J. Statistical power analysis for the behavioral
sciences. Hillsdale, NJ: Lawrence Erlbaum Associates 1998;
32. Power Analysis, Univresity of Visconsin Madison,
33. Grabowska B, Karaszewska A, Kamiska I. Badanie sztywnoci
zgina-nia dzianin osnowowych o strukturze siatki (in Polish). In:
IX Miedzynarodowa Konferencja Naukowo Techniczna Knitt Tech.
Received 14.03.2013 Reviewed 17.09.2013
INSTITUTE OF BIOPOLYMERS AND CHEMICAL FIBRES
LABORATORY OF BIODEGRADATION
The Laboratory of Biodegradation operates within the structure
of the In-stitute of Biopolymers and Chemical Fibres. It is a
modern laboratory with a certificate of accreditation according to
Standard PN-EN/ISO/IEC-17025: 2005 (a quality system) bestowed by
the Polish Accreditation Centre (PCA). The laboratory works at a
global level and can cooperate with many institu-tions that
produce, process and investigate polymeric materials. Thanks to its
modern equipment, the Laboratory of Biodegradation can maintain
coopera-tion with Polish and foreign research centers as well as
manufacturers and be helpful in assessing the biodegradability of
polymeric materials and textiles.
The Laboratory of Biodegradation as-sesses the susceptibility of
polymeric and textile materials to biological degradation caused by
microorganisms occurring in the natural environment (soil, compost
and wa-ter medium). The testing of biodegradation is carried out in
oxygen using innovative methods like respirometric testing with the
continuous reading of the CO2 delivered. The laboratorys modern
MICRO-OXYMAX RESPIROMETER is used for carrying out tests in
accordance with International Standards.
The methodology of biodegradability testing has been prepared on
the basis of the following standards:
n testing in aqueous medium: Determination of the ultimate
aerobic biodegrability of plastic materials and textiles in an
aqueous medium. A method of analysing the carbon dioxide evolved
(PN-EN ISO 14 852: 2007, and PN-EN ISO 8192: 2007)
n testing in compost medium: Determination of the degree of
disinterga-tion of plastic materials and textiles under simulated
composting condi-tions in a laboratory-scale test. A method of
determining the weight loss (PN-EN ISO 20 200: 2007, PN-EN ISO 14
045: 2005, and PN-EN ISO 14 806: 2010)
n testing in soil medium: Determination of the degree of
disintergation of plastic materials and textiles under simulated
soil conditions in a laborato-ry-scale test. A method of
determining the weight loss (PN-EN ISO 11 266: 1997, PN-EN ISO 11
721-1: 2002, and PN-EN ISO 11 721-2: 2002).
The following methods are applied in the as-sessment of
biodegradation: gel chromatography (GPC), infrared spectroscopy
(IR), thermogravi-metric analysis (TGA) and scanning electron
INSTITUTE OF BIOPOLYMERS AND CHEMICAL FIBRESul. M.
Skodowskiej-Curie 19/27, 90-570 d, Poland
Agnieszka Gutowska Ph. D., tel. (+48 42) 638 03 31, e-mail: